advertisement

Folding of Fiber Composites with a Hyperelastic Matrix Francisco López Jiménez, Sergio Pellegrino∗ Graduate Aerospace Laboratories, California Institute of Technology, 1200 E. California Blvd., Pasadena CA 91125 Abstract This paper presents an experimental and numerical study of the folding behavior of thin composite materials consisting of carbon ﬁbers embedded in a silicone matrix. The soft matrix allows the ﬁbers to microbuckle without breaking and this acts as a stress relief mechanism during folding, which allows the material to reach very high curvatures. The experiments show a highly nonlinear moment vs. curvature relationship, as well as strain softening under cyclic loading. A ﬁnite element model has been created to study the micromechanics of the problem. The ﬁbers are modeled as linear-elastic solid elements distributed in a hyperelastic matrix according to a random arrangement based on experimental observations. The simulations obtained from this model capture the detailed micromechanics of the problem and the experimentally observed nonlinear response. The proposed model is in good quantitative agreement with the experimental results for the case of lower ﬁber volume fractions but in the case of higher volume fractions the predicted response is overly stiﬀ. Keywords: ﬁber composites, hyperelastic matrix, bending, microbuckling, strain softening, random microstructure ∗ Corresponding author. Email address: [email protected] (Sergio Pellegrino) Preprint submitted to International Journal of Solids and Structures September 8, 2011 1. Introduction Deployable space structures have traditionally been based around stiﬀ structural members connected by mechanical joints, but more recently joint-less architectures have been proposed. In this case large relative motions between diﬀerent parts of a structure are achieved by allowing the connecting elements to deform elastically. For example, deployable solar arrays consisting of sandwich panels connected by tape spring hinges make use of cylindrical thin shells to provide the connection between the panels. This connection becomes highly compliant when elastic folds are created in the tape springs, allowing the panels to stow compactly, but it becomes much stiﬀer when the tape springs are allowed to deploy and snap back into the original conﬁguration. The maximum curvature of the tape springs cannot exceed a limiting value that is related to the failure strain of the material (Rimrott, 1966; Yee, Soykasap and Pellegrino, 2004). Tape spring hinges have been made from metal (Watt and Pellegrino, 2002; Auternaud et al., 1993), carbon ﬁber composites (Yee, Soykasap and Pellegrino, 2004; Yee and Pellegrino, 2005), and memory matrix composites (Campbell et al., 2005; Barrett et al., 2006). This last approach makes use of polymers that become softer above a transition temperature and these materials have been exploited to make hinges that can be heated and folded to very high curvatures. When they are cooled the hinges remain “frozen” in the folded conﬁguration but will then self-deploy when they are re-heated. A variant of this approach is to use a very soft elastic matrix, orders of magnitudes softer than standard epoxies; in this way the same type of behavior can be achieved without the need to heat the material. The reason is that the ﬁbers on the compression side of the material can form elastic microbuckles and so, instead of being subject to a large compressive strain, they are mainly under bending. This approach has already been exploited by Datashvili et al. (2010) who used a silicone matrix and by Mejia-Ariza et al. (2006) and Rehnmark et al. (2007) who used other approaches. Models showing exceptional folding capabil- 2 ities have been demonstrated (Datashvili et al., 2010; Mejia-Ariza et al., 2010). A number of simpliﬁed analytical models of this behavior have been already developed, see Section 2 of this paper, however these models do not capture the detailed micromechanics of the ﬁbers and matrix and so their predictive capability is limited. Our long-term objective is to establish experimentally validated models for the folding behavior of a thin composite consisting of unidirectional carbon ﬁbers embedded in a silicone matrix. Such models would be used to predict the strain in the ﬁbers for any given, overall curvature and hence to estimate the failure curvature of any specimen with known properties and to study a variety of related eﬀects, such as estimating the bending stiﬀness of a composite of stiﬀ ﬁbers embedded in a soft matrix, allowing for the softening associated with microbuckling. A key question that arises when developing such models is what assumptions are justiﬁed to reach an eﬀective compromise between model complexity and ability to obtain physically representative predictions. In the present study we focus on two key eﬀects, ﬁber distribution and large strain hyperelastic behavior of the matrix without any damage or other dissipation sources. Damage eﬀects have been considered in a separate paper (Lopez Jimenez and Pellegrino, 2011). The paper is laid out as follows. Section 2 presents a review of some relevant literature. Section 3 details the material properties and fabrication process, as well as an analysis of ﬁber distribution based on micrographs of actual specimens. Section 4 presents the experimental results of a folding test that shows evidence of microbuckling in the material; a characterization of the non-linear moment-curvature relationship of the material is also obtained. It is shown that, in addition to ﬁber microbuckling, there is evidence of damage-related stresssoftening. Section 5 describes the ﬁnite element model used to study in detail the behavior of a periodic unit cell based on a representative volume element (RVE) including a small number of elastic ﬁbers, typically between ten and thirty, embedded in a hyperelastic matrix. The RVE has a length longer than the buckle wavelength. Section 5.2 discusses two diﬀerent ﬁber arrangements used in the simulations. The ﬁrst one is a hexagonal pattern, characterized 3 only by the ﬁber volume fraction in the material. The second starts from a random distribution of ﬁbers that is rearranged until it matches the distribution observed in actual micrographs. The predictions for buckle wavelength and moment-curvature relationship obtained from the ﬁnite element model are compared with the experimental results in Section 6. Section 7 summarizes the ﬁndings of this work and concludes the paper. 2. Background The literature relevant to the present study can be categorized under three main headings: elastic ﬁber microbuckling, large straining of soft materials with embedded ﬁbers, and strain softening. Regarding the ﬁrst topic, ﬁber microbuckling is a well known failure mode for composite materials, see the review in Fleck (1997). Rosen (1965) proposed a model based on the buckling of a beam on an elastic foundation; he assumed a sinusoidal shape for the buckled ﬁbers and compared the work done by the external forces with the strain energy in the system. He considered two diﬀerent buckling modes. In the ﬁrst one the matrix deforms in extension, while in the second one it shears. The second mode requires a lower critical load and it is therefore considered the preferred one. Rosen’s approach of treating the ﬁbers as beams on an elastic foundation has been used by several other authors to explore the eﬀects of material thickness, ﬁber volume fraction and type of load, see for example Drapier et al. (1996, 1999, 2001) and Parnes and Chiskis (2002). Microbuckling has been invoked as a stress relieving mechanism in thermoplastic and elastic memory composites that are subject to large bending curvatures (Campbell et al., 2004; Marissen and Brouwer, 1999; Murphey et al., 2001). Figure 1 shows a sketch that explains this behavior. When folding starts, the extensional stiﬀness is uniform through the thickness and hence the neutral axis lies in the middle plane. As the ﬁbers on the compression side reach the critical buckling load, their stiﬀness is reduced in the post-buckling range and this corresponds to a bilinear constitutive model that shifts the neutral axis towards 4 the tensile side of the laminate. This eﬀect reduces both the maximum tensile and the maximum compressive strain in the ﬁbers, allowing them to remain elastic for much higher curvatures than if the ﬁbers had remained unbuckled. It should be noted that in Fig. 1 the buckling deﬂection has been depicted as out of plane for a better visualization, but experimental observations show that in most cases it occurs within the plane of the material, that is, parallel to the axis of bending. Stress Profile lo = π (r + t 2 ) ε= Tensile Stresses s lo − li π (r + t 2 )− π (r − t 2 ) t = = l r πr t l =πr Compressive Stresses Neutral Axis li = π (r − t 2 ) Figure 1: Fiber microbuckling and stress proﬁle in a heavily bent laminate, taken from Murphey et al. (2001). This eﬀect has been studied by Francis and co-workers (Francis et al., 2006; Francis, 2008) who provided the following approximation for the ﬁber buckle wavelength: λ= π 2 14 9Vf t2 d2 Ef ( √ ) Vf 8Gm ln 6t d π (1) where d is the ﬁber diameter, t is the thickness of composite plate being bent, Ef is the stiﬀness of the ﬁbers, Gm is the shear modulus of the matrix, and Vf is the ﬁber volume fraction. The amplitude of the buckle waves can be obtained from a= 2λ √ κ(z − zn ) π 5 (2) which relates the geometry of the buckled state with the applied curvature κ and the distance to the neutral axis z − zn . The maximum strain in the ﬁbers can then be obtained with: |ϵf | = d daπ 2 d κf = v′′ = 2 2 2λ2 (3) Studies of elastic memory composites (Campbell et al., 2005; Schultz et al., 2007) and also of carbon-ﬁber composites with a silicone matrix (Lopez Jimenez and Pellegrino, 2009) have extended Rosen’s model and all assumed small strains and a linear constitutive relationship both for the ﬁbers and the matrix. Turning to the second topic, large strain formulations for ﬁber reinforced composites were investigated by Merodio and Ogden (2002, 2003). Their model, based on Spencer (1972), introduces two invariants to model the eﬀect of the incompressible ﬁbers on the strain energy of the material. Following Geymonat et al. (1993), the appearance of macroscopic instabilities is related to the loss of ellipticity of the homogenized constitutive relationships. Several biological materials, such as the cornea or blood vessels, ﬁt the description of stiﬀ ﬁbers in a very soft matrix and models based on such an approach have been used by Holzapfel et al. (2000); Pandolﬁ and Manganiello (2006); Pandolﬁ and Holzapfel (2008). The second order homogenization theory developed by Ponte Castañeda (2002) has also been applied to ﬁber-reinforced hyperelastic materials. This approach is still under development, see for example Lopez-Pamies and Ponte Castañeda (2006), Agoras et al. (2009) and Lopez-Pamies and Idiart (2010); a comparison to numerical results has been presented in Moraleda et al. (2009b). In all of these studies the loading is two dimensional, usually under the assumption of plane strain. To the authors’ knowledge, there is no detailed experimental or theoretical analysis of ﬁber reinforced soft materials under bending, which is the situation most relevant to the present study. The ﬁnal topic is strain softening, of a type known to occur in particle reinforced rubbers, such as tires. Their behavior is shown schematically in 6 Figure 2. If a virgin material sample is loaded to the strain level (1) it follows the path (a), known as the primary loading curve. Subsequent unloading and loading to (1) will follow the path (b) as the material has been weakened by the initial loading process and so its stiﬀness is reduced. If the strain exceeds (1) path (a) is joined again. If unloading from a higher strain level (2) occurs, it will create a new path (c) with an even greater loss of stiﬀness. This type of behavior is usually called Mullins’ eﬀect. Figure 2: Schematic of cyclic tension demonstrating Mullin’s eﬀect. Taken from Govindjee and Simo (1991). The process described above is somewhat idealized as in reality there is a stress reduction on each successive loading and unloading cycle. The reduction is largest between the ﬁrst and second cycle, and it becomes very small after a few cycles, a process known as preconditioning. After these initial cycles the stress-strain response is essentially repeatable. Representing the loading and unloading path as coincident is also an idealization. There are large diﬀerences in the stress in both states, even in rubbers not showing hysteresis before being reinforced. All these phenomena depend on the concentration of particles in the rubber. In particular, both the softening and the hysteresis increase with the ﬁller content. Several models for stress-softening have been proposed, see for example Govindjee and Simo (1991) or Dorfmann and Ogden (2004). Stress softening is also common in biological tissues, including tissues composed of collagen ﬁbers in soft matrix (Fung, 1972; Holzapfel et al., 2000). In 7 general, stress softening can be eliminated by preconditioning the material. 3. Specimen Fabrication and Characterization 3.1. Fabrication The ﬁbers were HTS40-12K, produced by Toho Tenax (retrieved August 2010) and provided by the Itochu Corporation in the form of a uniaxial ply of dry ﬁbers with an areal density equal to 40 g/m2 . This implies that every 12K tow has been spread to a width of approximately 20 mm, although the separate tows are almost indistinguishable. The properties of the ﬁbers are provided in Table 1; note that only longitudinal properties were obtained. Comparative studies using typical values for the remaining properties were performed in Section 5.1 . Fiber properties Diameter 7 µm Longitudinal modulus 240 GPa 1.77 g/cm3 Density Strain at failure 1.8% Matrix properties Viscosity (part A) 1300 mPa s Viscosity (part B) 800 mPa s Density 0.96 g/cm3 Tensile modulus 0.8 MPa Strain at failure 100% Table 1: Material properties provided by the manufacturers The matrix material was CF19-2615, produced by NuSil Silicone Technology (March 2007). This is a two part, optically clear silicone chosen for its low viscosity (see Table 1) in order to facilitate its ﬂow within the ﬁbers. The fabrication process was as follows. First the two parts of the silicone were mixed, then vacuum was applied to extract air bubbles and ﬁnally the 8 mixture was poured over the ﬁbers, previously placed on either a Teﬂon coated tray for the case of specimens cured in an oven or on a PTFE sheet for specimens cured in an autoclave. Both types of specimens were cured for 30 minutes at 150◦ C. In the case of autoclave curing the specimens were vacuum bagged, so internal vacuum and up to 85 psi (0.586 MPa) of external pressure were applied. Deﬁning the ﬁber volume fraction as Vf = Af A (4) where Af is the cross sectional area of the ﬁbers and A is the total area of the cross section, both observed in a micrograph, autoclave curing is able to better control Vf and hence to achieve values between 25% and 55%, see Figure 3. Holding the specimen under vacuum is the main contributor to achieving specimens with a homogeneous ﬁber distribution. Increasing the pressure diﬀerential has the advantage of better consolidating the ﬁbers and also achieving a more homogeneous distribution of ﬁbers in the matrix. Fiber volume fraction (%) 60 55 50 45 One ply Two plies Three plies 40 35 0 0.1 0.2 0.3 0.4 0.5 Differential pressure (MPa) 0.6 Figure 3: Average ﬁber fraction vs. diﬀerential pressure applied during curing. The ﬁber volume fraction is fairly independent of the amount of silicone poured over the ﬁbers. In composites cured in the autoclave, the diﬀerential pressure is enough to evacuate the extra silicone through a perforated release 9 ﬁlm. In specimens cured in the oven it is possible to obtain overall values of Vf even lower than 25% by applying an excess of silicone, but this does not result in a homogeneous distribution of the ﬁbers. An extreme case (Vf ≈ 10% ) can be seen in Figure 4 where it should be noted that most of the ﬁbers have concentrated in a narrow region and are surrounded by pure silicone. The local ﬁber volume fraction in the region containing the ﬁbers is approximately 25%. Figure 4: Specimen with Vf = 10% overall, showing a high degree of ﬁber localization in the middle. 3.2. Characterization of Fiber Geometry One of the goals of the numerical models presented in this paper is to study the inﬂuence of simulating a realistic ﬁber arrangement, as opposed to regularly arranged ﬁbers. In order to produce such a model it is necessary to obtain micrographs of the material cross section. In composites with a harder matrix the micrographs would be obtained from specimens with a ﬂat and smooth surface, but this is not possible in the case of a very soft matrix. Instead, the material was cut with a razor blade and then placed under a Nikon Eclipse LV100 microscope with 50x ampliﬁcation and a Nikon DS-Fi1 digital camera. The surface obtained this way is not suﬃciently ﬂat to lie entirely within the depth of ﬁeld of the microscope. In order to obtain a sharp image several 10 pictures of the specimen were taken at diﬀerent focus distances and the pictures were then processed with the focus stacking capabilities of Adobe Photoshop CS4 (Adobe Photoshop CS4, 2008), see Figure 5. Figure 5: Micrograph obtained by stacking six images in Photoshop, Vf = 30%. The micrographs can be used to verify measurements obtained with less precise techniques. The ﬁber volume fraction and thickness observed were the same as those calculated by measuring the dry weight of the ﬁbers and the weight of the cured specimen. The micrographs show that there are 0.63 ﬁbers per micrometre of width, which agrees with the value calculated from the weights. The position of the ﬁbers within the micrographs was recorded in order to obtain a statistical characterization of their arrangement. In general, the ﬁber arrangement can be described by the radial distribution function (RDF) which is commonly used to characterize statistically isotropic particle systems. The RDF measures the probability of ﬁnding a ﬁber at a given distance from the center of another ﬁber. Rintoul and Torquato (1997) have shown that the RDF is suitable to reconstruct systems with low particle densities, or systems with high densities in which the particles have no tendency to aggregate. The micrographs show that this is the case for the present material. The RDF is properly deﬁned for systems that are isotropic in all dimensions, and normalized so that it tends to one as r tends to inﬁnity. In the present case the composite material is better idealized as a strip that is only isotropic in one dimension. Instead of using the RDF, the second-order intensity function K(r) (Pyrz, 1994a,b) was used. K(r) is deﬁned as the number of ﬁbers expected to 11 lie within a radial distance r from an arbitrary ﬁber, normalized by the overall ﬁber density. It is proportional to the integral over the radius of the RDF, and the two functions provide the same information. Figure 6 shows the average number of neighbor ﬁbers as a function of distance for samples with two diﬀerent values of Vf , as well as the corresponding second-order intensity function. 25 2 Vf = 30 % V = 30 % f 1.8 Vf = 55 % 20 V = 55 % f 1.6 15 K(r) x 103 Number of fibers 1.4 10 1.2 1 0.8 0.6 5 0.4 0.2 0 2 4 6 Distance / fiber radius 0 2 8 4 6 Distance / fiber radius 8 Figure 6: Average number of ﬁbers as a function of distance from a given ﬁber: (a) total number of ﬁbers and (b) second-order intensity function. 4. Experiments 4.1. Silicone Rubber The modulus and elongation properties in Table 1 were veriﬁed experimentally through uniaxial testing. Two diﬀerent set of values were found, see Figure 7. For specimens cured in the autoclave, failure typically occurred at 120140% elongation, with a value of the Cauchy stress of approximately 1.25 MPa. For specimens cured in the oven the values were 100-120% and 1.7 - 2 MPa, respectively. It is believed that the reason for the diﬀerence is the presence of epoxy residue in the autoclave, where traditional composites are often cured. 12 Cauchy stress (MPa) 2 Cured in autoclave Cured in oven 1.5 1 0.5 0 1 1.5 2 λ Figure 7: Uniaxial stress-stretch relationship of CF19-2615 silicone. The two specimens are taken from the same batch of silicone, the only diﬀerence being the curing. Figure 8 shows the stress-stretch and stress-time relationship obtained from tests combining cyclic and relaxation loading. These results show negligible hysteresis or viscoelastic eﬀects, which agrees with published test results for silicone rubber (Meunier et al., 2008; Machado et al., 2010). Other types of rubbers exhibit strain softening even when they are unreinforced. 4.2. Folding Tests The specimens were put in a ﬁxture that imposes a 90◦ kink angle and a radius of curvature of approximately 2 mm. Figure 9 shows the tension and compression side of a specimen with Vf = 30%. Microbuckling can be observed; buckles appear both on the compression and tension sides, but the buckle amplitude is larger on the compression side. This observation agrees with the simulation results shown in Section 6. The experiment was repeated on a specimen with Vf = 55% and similar images were obtained in this case. The existence of buckled ﬁbers on the tension side is typical of very thin composites and does not happen in the case of thicker specimens (Francis, 2008). 13 Cauchy stress (MPa) Cauchy stress (MPa) 2 1 0 1 1.2 1.4 1.6 λ 1.8 2 2.2 2 1 0 0 2000 4000 6000 Time (s) 8000 10000 Figure 8: Uniaxial stress-stretch and stress-time relationship for silicone, obtained from a test involving cyclic loading with holding periods; the silicone had been cured in an oven. 4.3. Bending Test Setup Standard methods to measure the bending stiﬀness, such as the four point bending test, are limited to relatively stiﬀ specimens that undergo only small curvatures. In order to measure the non-linear moment-curvature relationship at larger curvatures a diﬀerent technique is required. In this study the momentcurvature relationship was obtained from the post-buckling behavior of specimens under compressive load. 9 to 15 mm wide specimens were sandwiched between 0.6 mm thick Aluminiumalloy plates. The plates were glued to the specimens with Instant Krazy Glue, leaving a 4 mm distance between the two pairs of plates, see Figure 10, (a). The sandwiched ends of these specimens are much stiﬀer than the composite-only strip in the middle and so they can be idealized as rigid. To reduce the eﬀects of friction and contact the plates were connected with Scotch Magic Tape to rigid blocks attached to the jaws of a materials testing machine (INSTRON 5569 with a 10 N load cell), see Figure 10, (b). Note 14 1 mm a b Figure 9: Specimen with Vf = 30% folded 90◦ with a 2 mm radius: (a) view of outside of fold region, i.e. tension side of specimen and (b) view of inside of fold region, i.e. compression side of specimen. 15 a aluminum plates specimen b c L δ b h Wd 2h F-W/2 M W/2 F d F L Wd 2h M W/2 F+W/2 Figure 10: Test for high curvature bending: (a) preparation of specimen, (b) test setup, showing bending of specimen due to compressive displacement and (c) analysis of geometry and force equilibrium in the test. 16 that the specimen does not touch the blocks at any point during the test: it is connected solely to the tape. The bending stiﬀness of the tape is much lower than that of the specimen and therefore this connection can be treated as a zero-moment hinge. The specimens were weighted before the test; their total weight, W , including the aluminum plates was approximately 1 gram. A schematic analysis of the test is shown in Figure 10(c). The vertical displacement δ = 2L + b − 2h is controlled and the corresponding vertical load measured by the load cell is F − W 2 , where F is the vertical force at the center of the specimen. Assuming a uniform curvature, κ, in the specimen the main geometric parameters can be expressed as: κ= 2θ b b sin θ 2θ (6) b (1 − cos θ) 2θ (7) h = L cos θ + d = L sin θ + (5) Hence κ can be calculated from the vertical displacement, measured by the testing machine. The assumption of uniform curvature implies that the moment is uniform within the compliant part of the specimen, and equal to: ( ) W M= F− d 4 (8) This result is valid when the length of the composite-only strip is small compared to the length of the end plates, b << L; in the present case b = 4 mm and L = 25.4 mm. This assumption was checked by comparing the results to a more exact solution using non-uniform curvature: no diﬀerence could be observed. Photos of the specimens during the tests also showed uniform curvature. Neglecting the weight W , the maximum normal stress due to the force F , σF , and the maximum stress due to the bending moment, σM , can be found 17 from simple beam theory σF = σM = F bt Mt 6F d = 2 2I bt (9) (10) where t is the thickness, b the width, and I the second moment of area of the specimen. From these two equations we ﬁnd that σF and σM are related by σM = σF 6d t (11) and for the geometry of the present test σM is 300 to 500 times larger than σF . For this reason, the eﬀect of F can be neglected and the test treated as applying a pure bending moment. Table 2 shows the typical dimensions of the specimens used during the tests. Length, b 4 mm Width 9 - 15 mm Thickness - 55% Vf 45 µm Thickness - 30% Vf 75 µm Table 2: Dimensions of bending test specimens 4.4. Bending Test Results The results of two sets of bending tests are shown in Figures 11 and 12. Each test consisted of three cycles with increasing maximum curvature of 0.22, 0.30 and 0.36 mm−1 and each cycle was repeated four times. There are clear signs of strain induced stress softening associated with damage; this behavior is discussed in more detail in Lopez Jimenez and Pellegrino (2011). In this paper we will focus on the loading part of the ﬁrst cycle in Figures 11(a) and 12(a), during which the maximum moment value was attained by each specimen. For both specimens the ﬁrst monotonic loading momentcurvature relationship is approximately linear for low curvatures. At approximately 0.07 mm−1 the stiﬀness starts decreasing and for higher curvatures the slope becomes negative. 18 The tests were performed at three diﬀerent speeds: 0.25, 0.5 and 1 mm/min of vertical displacement. Note that a uniform vertical displacement rate δ̇ does not translate into a uniform curvature rate κ̇. Assuming that b << L, the relationship between the two is given by κ̇ = 2δ̇ Lb sin θ (12) For example, the test geometry show that a uniform vertical displacement rate of 1 mm/min corresponds to curvature rates varying between 0.05 and 0.25 mm−1 once the specimen has microbuckled. No signiﬁcant diﬀerences were found and hence rate dependence eﬀects were neglected. The same two specimens were tested again 24 hours after the ﬁrst test and the results are shown in Figures 11(b) and 12(b). The damage was not recovered and the stiﬀness was the same as at the end of the previous test. Both the permanent loss of stiﬀness and the cycle hysteresis are less pronounced in specimens with lower ﬁber volume fraction. This observation agrees with the typical behavior of particle reinforced rubbers discussed in Section 2. 5. Finite Element Analysis 5.1. Model A micromechanical ﬁnite element model of a bending specimen was set up in the ﬁnite element package Abaqus/Standard (Abaqus/Standard, 2007) where both matrix and ﬁbers were modeled with 3D solid elements. Initial attempts to model the ﬁbers with 1D beam elements did not produce useful results, as it is impossible to correctly model the volume fraction of the material and so the stress distribution turns out to be vastly incorrect. The use of 3D elements is required to preserve the geometry of the problem. Bonding between matrix and ﬁbers was assumed to be perfect and therefore both materials share the nodes lying on the contact surfaces. To reduce the computational cost only a repeating RVE of a tow was modeled: in a study of a tow under bending this RVE must extend through the 19 Moment per unit width (N) 0.025 0.025 0.02 0.02 0.015 0.015 0.01 0.01 0.005 0.005 0 0 0.1 0.2 0.3 0.4 0 0 0.1 -1 0.2 0.3 0.4 -1 Curvature (mm ) Curvature (mm ) = 0.22 mm -1 a -1 = 0.30 mm = 0.36 mm -1 b Figure 11: Moment-curvature relationship for a specimen with Vf = 55%, showing strain softening under cycling loading: (a) initial test and (b) test repeated on same specimen after Moment per unit width (N) 24 hours. 0.045 0.045 0.04 0.04 0.035 0.035 0.03 0.03 0.025 0.025 0.02 0.02 0.015 0.015 0.01 0.01 0.005 0.005 0 0 0.1 0.2 0.3 0.4 0 0 -1 0.1 0.2 0.3 0.4 -1 Curvature (mm ) Curvature (mm ) = 0.22 mm a -1 = 0.30 mm -1 = 0.36 mm -1 b Figure 12: Moment-curvature relationship for a specimen with Vf = 30%, showing strain softening under cycling loading: (a) initial test and (b) test repeated on same specimen after 24 hours. 20 whole thickness of the tow. Deﬁning the x-axis in the direction of the ﬁbers and the y-axis perpendicular to the mid-plane of the tow, we considered RVE’s resulting from cutting the tow with two planes parallel to the xy plane and at distance W , as seen in Figure 13. The RVE has length L, width W and height H, as deﬁned in the ﬁgure. The arrangement of the ﬁbers within the cross section will be discussed in Section 5.2. Fiber z y Matrix x RVE L H W Figure 13: Representative volume element. The boundary conditions on the faces of this RVE must ensure periodic behavior in the z direction. Since the meshing of the two faces is identical, periodic boundary conditions were applied directly to corresponding nodes using the EQUATION command in ABAQUS. The displacement components in the x and y directions (u and v, respectively) of every node were forced to be equal to those of the corresponding node on the opposite face: u(x, y, 0) = u(x, y, W ) (13) v(x, y, 0) = v(x, y, W ) (14) The diﬀerence of displacements in the z direction (w) in each pair of nodes 21 has to be same. This implies that the width of the RVE may change with respect to the undeformed conﬁguration, but it has to be constant through the model: w(x1 , y1 , 0) − w(x1 , y1 , W ) = w(x2 , y2 , 0) − w(x2 , y2 , W ) (15) The analysis of a RVE is still computationally very expensive if one attempts to model the complete length b of the bending region in a specimen. Instead, it was decided to simulate a piece of material away from the boundaries. In order to achieve this, the only boundary condition that was applied at the end cross sections is the requirement that the nodes should remain coplanar. The relative position within the plane was left unconstrained, including the displacement in the z direction. The nodes lying in each of these planes were connected to a dummy node, one for each face. Equal and opposite rotations about z, of magnitude θ, were applied to each dummy node. One of the dummy nodes was constrained against translation in all directions, while the other one was left free to translate along the x axis, in order to eliminate all remaining rigid body motions. The faces perpendicular to the y axis were left free. Müller (1987) showed that the use of RVE’s does not ensure ﬁnding the correct solution in problems of nonlinear elasticity, such as buckling. Instead, all possible combinations of RVEs should be considered and analyzed. The correct solution is the one corresponding to the lowest energy in the system. This approach has been explored in works studying the non-linear behavior of composite materials, such as buckling of laminates under plane strain (Geymonat et al., 1993). For the model presented here, Müller (1987)’s result implies that the use of a RVE will neglect all possible instabilities with wavelength longer than the size of the cell. This would be a problem if the wavelength of the simulated instability was the same as the length of the model, in which case it is possible that using a larger model would result in a longer wavelength. However, the results presented in Section 6 show that the models used in the present study are able to capture at least half the length of a sinusoidal buckle. Since the minimum 22 wavelength that can be captured by this model is a quarter of a buckle, the length of the model should not aﬀect the computed response. Regarding the number of ﬁbers, models with up to 33 ﬁbers have been used. No diﬀerence with respect to smaller models was observed. This suggest that there are no instabilities dependent on the z coordinate. Such instabilities have not been observed experimentally, either. Therefore it is unlikely that the model neglects an important deformation mechanism due to insuﬃcient width. The ﬁbers were modeled as a linear elastic material, since the maximum ﬁber strains observed during the simulations were lower than 1%. The elements used were the solid triangular prisms C3D6 and the material was deﬁned as isotropic since a full orthotropic description of the ﬁbers was not available. Still, a model including ﬁve ﬁbers in the RVE was used to perform a comparative study, using typical properties of carbon ﬁbers where no speciﬁc data could be found, such as 20 GPa for the orthotropic stiﬀness. This analysis showed that the main eﬀect of modeling the ﬁbers as orthotropic is a small reduction in the overall bending stiﬀness. To obtain some preliminary results the matrix was initially modeled as a linear elastic material but the high strain concentrations, with values of up to 50% even at the initial stages of buckling, made this model numerically unstable even for small applied curvatures. The matrix was then modeled as an incompressible rubber. The elements used were the hybrid square prisms C3D8H. The use of triangular prisms (C3D6 and higher order elements C3D15H) had produced locking due to incompressibility. Next, two diﬀerent hyperelastic potentials were used to model the matrix: the Ogden model (Ogden, 1972), implemented in ABAQUS as one of the standard material models for rubber, and the model provided by Gent (2005). The second model provided a better ﬁt for the experimental data for the same number of parameters, and hence was adopted for the simulations. The Gent model was implemented in ABAQUS as a user deﬁned material, 23 using the user subroutine UHYPER. The hyperelastic potential is given by: ( ) ( ) J1 J2 + 3 W = −C1 Jm ln 1 − + C2 ln Jm 3 (16) J1 = λ21 + λ22 + λ23 − 3 (17) −2 −2 J2 = λ−2 1 + λ2 + λ 3 − 3 (18) where and C1 , C2 and Jm are parameters to be determined. These parameters were obtained by ﬁtting data to the uniaxial tests presented in Section 4.1. The values obtained were C1 = 0.1015 mJ, C2 = 0.1479 mJ and Jm = 13.7870 for the specimens cured in the autoclave and C1 = 0.1303 mJ, C2 = 0.1345 mJ and Jm = 6.3109 for those made in the oven. It must be noted that the strain energy tends to inﬁnity when J1 = Jm . In a uniaxial tension state and for the parameters used in the present study this happens for a value of the elongation well beyond the failure stretch. However, this condition is not implemented in the model and, even if such large values are not reached, the simulation might still need to use them in the middle of an equilibrium iteration. In order to prevent numerical errors the ﬁrst term in the strain energy equation was substituted by a quadratic function of J1 . The resulting expression is continuous up to the second derivative: W ( ) J1 = −C1 Jm ln 1 − Jm ( ) J2 + 3 + C2 ln 3 24 (19) if J1 ≤ 0.9Jm W C1 (J1 − 0.9Jm ) 0.1 2 J1 (J1 − 0.9Jm ) + 0.5 0.01Jm ) ( J2 + 3 + C2 ln if J1 > 0.9Jm 3 = −C1 Jm ln(0.1) + (20) The most obvious implication of this modiﬁcation is that the model is stiﬀer than the real material once the strains in the matrix go beyond the point at which the material should have actually failed. In reality, damage would occur at such large strains, and hence this is a limitation of the present model. 5.2. Arrangement of fibers Two diﬀerent approaches to the distribution of ﬁbers in the material were investigated. In the ﬁrst approach, the ﬁber axes form an hexagonal grid with a spacing that matches the overall Vf measured from the micrographs. The width of the RVE is such that it contains a column of complete ﬁbers as well as two columns of half ﬁbers (Figure 14) and the resulting geometry is provided in Table 3. Volume fraction 55% 30% Number of ﬁbers 9 13 Distance between ﬁbers 8.99 µm 12.17 µm Height (H) 40.4 µm 79.1 µm Width (W) 15.6 µm 21.1 µm Table 3: Dimensions of hexagonal RVE’s. The hexagonal lattice is a common idealization of ﬁber distributions but micrographs of the material show it is an unrealistic one. Since the ﬁbers are expected to undergo very large deﬂections the strain energy in the matrix will greatly depend on the spacing between ﬁbers. Random distributions of ﬁbers have been used in works studying the nonlinear deformation of composites under plane strain (Moraleda et al., 2009a,b). Although more realistic, 25 this approach still does not ensure that the geometry of the real material is fully captured. With this objective, a reconstruction based on the approach presented in Rintoul and Torquato (1997) was adopted. The main three steps of the algorithm are presented next. 5.2.1. Initial location of fibers The number of ﬁbers to be placed in the RVE is calculated according to the volume fraction. The ﬁbers are ﬁrst allocated randomly within the RVE. For a ﬁber to be accepted, it cannot be closer than a given value from any of the previously accepted ﬁbers. Otherwise it is discarded, and a new random location is produced. If no suitable location has been found after 1000 attempts, the ﬁber is accepted anyhow; this limit to the number of attempts is necessary since in cases with Vf > 50% the process is likely to reach a jamming situation before all the ﬁbers are placed. The minimum distance that needs to be enforced is obviously twice the radius of the ﬁbers. In the present case the value used was 8 µm, that is 1 µm higher than the ﬁber diameter, to ensure that the matrix between the ﬁbers can be meshed adequately. If the distance from the center of a ﬁber to the side in which periodic boundary conditions are applied is less than a ﬁber radius, then a symmetric ﬁber must be placed on the other side of the RVE, to satisfy the periodicity of the RVE. In order to avoid poor meshes, ﬁbers whose surface is closer than 1 µm to the edges of the RVE are discarded. 5.2.2. Potential energy Once all the ﬁbers have been placed, a potential energy E is deﬁned. It will be used to quantify the diﬀerence between the current conﬁguration and the goal one, based on several micrographs of the specimen that is being studied. The function used for the reconstruction is the second-order intensity function presented in Section 3.2. The potential is deﬁned as: E= ∑( 2 K (ri ) − (K0 (ri )) ) + ∑ j i 26 (M δj ) (21) where K0 is the second-order intensity function observed in the micrographs, the summation in i is made over the intervals used to discretize r, M is a large positive number and δi is equal to one if the j-th ﬁber violates one of the rules explained before (such as intersecting with another ﬁber) and zero otherwise. 5.2.3. Evolution process A ﬁber is picked randomly and a random displacement is applied. The potential E ′ is calculated for this new conﬁguration. If it is lower than the previous value, the displacement is accepted. If it is higher, the displacement is accepted with probability e E−E ′ A , where A is a parameter that controls how fast the system should evolve (a value of 0.05 has been used in this work). This means that the algorithm would accept some of the displacements in which the energy increases slightly, but almost none implying a large increment. This last step is repeated until the system converges to a stable value of E. Figure 14 shows the hexagonal RVE corresponding to Vf = 55% as well as two examples of random arrangements. The ﬁrst random cell has the same width as the cell obtained with the hexagonal pattern, while the second one is 50% wider. In the case Vf = 55% no dependence on the size of the RVE was observed. By contrast, the width of the specimens was found to be important in the case of lower volume fractions. The reconstruction process tends to group the ﬁbers in clusters, leaving large regions of pure silicone. For example, the reconstruction process might produce a RVE such as that in Figure 15(b) and, because of the periodic nature of our model, there will be a band without ﬁbers extending through the whole model. It is possible to produce RVE’s with the same size that do not present such problems, Figure 15(c), although the process has a better outcome with wider RVE’s, see Figure 15(d). The random RVE’s used in this work have up to two and half times the thickness of those with hexagonal pattern, which corresponds to roughly 30 ﬁbers. 27 a c b Figure 14: Examples of RVE’s with Vf = 55%: (a) hexagonal pattern; (b) random RVE with the same width as (a); and (c) random RVE with 1.5 times the width of (a). a b c d Figure 15: Examples of RVEs with Vf = 30%: (a) hexagonal pattern, (b) unrealistic random RVE with same width as (c); (b) realistic random RVE with same width as (a); and (d) realistic random RVE with 1.5 times width of (a). 28 6. Finite Element Results The results presented in this section were produced from models with typically 100,000 to 120,000 nodes and 120,000 to 150,000 elements. Analyses carried out with ﬁner meshes provided practically identical results, both in terms of macroscopic (wavelength, moment-curvature relationship) and microscopic (strain localization) features. 6.1. Deformed Geometry Figures 16 and 17 show diﬀerent views of the deformed conﬁguration obtained from one of the simulations (hexagonal pattern, Vf = 55%). All of the characteristic features of the folding of a ﬁber composite with a hyperelastic matrix can be seen in these results: in-plane buckling of the ﬁbers, large ﬁber deﬂections, larger buckle amplitude on the compression side and uniform curvature. These features are common to all cases, regardless of ﬁber arrangement and ﬁber volume fraction. The buckle wavelength ranges from 0.33 mm to 0.5 mm in the case shown (Vf = 55%) and 0.5 mm to 1 mm in the case Vf = 30%. a b Figure 16: Views of deformed conﬁgurations of RVE with hexagonal ﬁber arrangement, Vf = 55% and L = 1 mm subject to κ = 0.7 mm−1 : (a) side view and (b) top view. 29 Figure 17: Perspective view of RVE showing longitudinal stress ﬁeld. Vf = 55%, hexagonal ﬁber arrangement, 1 mm length, κ = 0.7 mm−1 . It should be noted that the wavelength computed from these simulations is aﬀected by the chosen length L of the RVE, which is 1 mm in all the cases considered. Changing L by a small amount would probably result in the same number of waves and therefore a diﬀerent wavelength. This eﬀect could be minimized by analyzing a much longer RVE, but this could not be done due to the already high computational cost of the present analysis. The wavelengths predicted by the simulations are shorter than those observed experimentally for Vf = 55%, although the predictions are much closer for for Vf = 30%, see Table 4. Analytical results in Francis (2008); Lopez Jimenez and Pellegrino (2009) show that as the wavelength increases the strain energy of the matrix also increases, while the strain energy of the ﬁbers decreases. The present results are therefore an indication that the ﬁnite length of the present model has not allowed the ﬁbers to form buckles of unconstrained length. 30 Volume fraction 55% 30 Simulations 0.33 - 0.5 mm 0.5 - 1 mm Experiments 0.55 - 0.70 mm 0.6 - 0.65 mm Table 4: Comparison of wavelengths from simulations and experiments. 6.2. Strains The evolution of the largest principal strains with the applied curvature can be studied with these models, see Figures 18 and 19. In the case Vf = 55% randomness in the ﬁber distribution does not lead to signiﬁcant changes in the maximum strains, since the ﬁbers are already densely packed even in the hexagonal arrangement. In the case Vf = 30% the maximum strains are higher in the case of random ﬁber arrangement. 8 x 10 -3 6 6 x 10 -3 4 4 2 Strain 2 0 0 -2 -2 -4 -4 -6 -8 0 0.2 -6 0.4 -1 a 0 0.2 0.4 -1 Curvature (mm ) Curvature (mm ) Hexagonal Random b Figure 18: Maximum and minimum principal strains in the ﬁbers: (a) Vf = 55% and (b) Vf = 30%. Since the buckled ﬁbers are mainly subjected to bending, the maximum and minimum principal strains give a very good indication of the possibility of failure 31 3 1.5 2 1 0.5 1 Strain 0 0 -0.5 -1 -1 -2 -1.5 -3 -4 -2 0 0.2 0.4 -1 -2.5 0 0.2 0.4 -1 Curvature (mm ) Curvature (mm ) a Hexagonal Random b Figure 19: Maximum and minimum principal strains in the matrix: (a) Vf = 55% and (b) Vf = 30%. in the material. The failure elongation of the ﬁbers in Table 1 is 1.8% and the predictions in Fig. 18 are well below this value. The strain state in the matrix is rather more complex and, since there are no established failure criteria for silicone rubber under multi-axial loading conditions, it is hard to tell what combination of strains or stresses in the matrix would cause failure. Damage processes such as cavitation, debonding between silicone and carbon ﬁbers (which will also depend on the type and amount of sizing used to coat the ﬁbers), breaking and disentanglement of polymer chains, etc. will play a role. Since the largest strains in the matrix provided by the simulations, in excess of 200%, are so much greater than the failure strain obtained from the uniaxial tensile tests in Section 4.1, damage would be expected to occur before reaching such high strains. Hence it can be concluded that our matrix model will tend to become unrealistically stiﬀer. The fact that the maximum principal strains in the matrix are similar for hexagonal and random arrangements of the ﬁbers does not mean that the strain 32 states are in fact similar. Figure 20 shows contour plots of γyz for two models with Vf = 55%. Both sections shown in this ﬁgure correspond to the point of maximum deﬂection of the buckle, for κ = 0.35 mm−1 . In the case of the hexagonal pattern all ﬁbers buckle together, the only diﬀerence being in the amplitude, and this produces a regular strain pattern in the matrix. The randomly arranged ﬁbers create a less regular strain distribution, with high positive and negative strains within the same section. In the latter case the amplitude of the buckle is practically the same through the whole thickness and this produces higher strains in both matrix and ﬁbers. yz +2.000 +1.250 +0.500 -0.250 -1.000 -1.750 -2.500 y z a b Figure 20: γyz strain ﬁeld for Vf = 55%: (a) hexagonal pattern and (b) random pattern. In the case of lower ﬁber volume fractions the results are similar for the random and regular ﬁber arrangements, see Figure 21. In particular, the variation of the ﬁber buckle amplitude through the thickness of the RVE is similar for both arrangements, unlike the previous case. Simulations based on RVE’s with a larger number of ﬁbers give similar results, the main diﬀerence being the presence of larger areas of pure silicone, in which the material can shear very easily, see Figure 22. The use of wider RVE’s tends to impose a more homogeneous variation of the buckled amplitude 33 yz +1.000 +0.550 +0.100 -0.350 -0.800 -1.250 -1.700 y z a b Figure 21: γyz strain ﬁeld for Vf = 30%: (a) hexagonal pattern and (b) random pattern. through the thickness. 6.3. Moment vs. Curvature The higher strains observed in the cases with random ﬁber arrangement correspond to a greater stiﬀness overall, as can be seen by plotting the momentcurvature relationship. In all plots the curvature is assumed to be uniform along the length of the model and it is therefore calculated by dividing by L the relative rotation applied at the ends. Figure 23 shows the moment-curvature relationship of the simulations with Vf = 55%. The cases with random ﬁber arrangement show some variation among each other, but they are clearly stiﬀer than the case with hexagonal pattern. An analysis with linear geometry for the hexagonal pattern is also plotted for comparison: it coincides with the initial response of all cases. Once the ﬁbers have buckled, the stiﬀness of the regular pattern drops to only about 20% of the initial stiﬀness, whereas in the case of randomly arranged ﬁbers the stiﬀness drops to 60 - 75 %. In the cases with Vf = 30% the response of the models with regular and random ﬁber arrangements are much closer to each other, and both of them are much softer than the linear prediction, see Figure 24. The sudden drop 34 yz +2.000 +1.333 +0.667 0 -0.667 -1.333 -2.000 y z Figure 22: γyz strain ﬁeld for Vf = 30%; the width is 2.5 times that of the RVE with hexagonal Moment per unit width (N) ﬁber arrangement. Linear Hexagonal pattern Random pattern 0.25 0.2 0.15 0.1 0.05 0 0 0.05 0.1 0.15 0.2 0.25 0.3 0.35 Curvature (mm−1) Figure 23: Moment vs. curvature for simulations with Vf = 55%. The plot shows the results from the simulation with hexagonal ﬁber arrangement, four simulations with random RVE’s, and a linear analysis for reference. 35 in stiﬀness is related to the sudden start of microbuckling, which is associated with a drop to a lower state of energy. This produces a discontinuity in the ﬁrst derivative of the strain energy. This is not likely to occur in the real material, due to the presence of imperfections that will produce a smooth transition to the buckled state. The eﬀect can be reduced by introducing waviness in the ﬁbers, but it is hard to make it disappear completely. Moment per unit width (N) 0.1 0.08 0.06 0.04 Linear Hexagonal pattern Random pattern 0.02 0 0 0.05 0.1 0.15 0.2 0.25 0.3 Curvature (mm−1) Figure 24: Moment vs. curvature for simulations with Vf = 30%. The plot shows the results from the simulation with hexagonal ﬁber arrangement, three simulations with random RVE’s, and a linear analysis for reference. The results of the ﬁnite element analysis and the experiments are compared in Figure 25 and Figure 26, where the area enveloped by the simulations with several diﬀerent initial geometries of random ﬁbers has been shaded in grey. In the ﬁrst case, Vf = 55%, the prediction is much stiﬀer than the actually measured behavior. It is believed that there are two main reasons. The ﬁrst one is the extreme strain concentrations in the silicone, as shown earlier in the paper, which would case localized failures; these eﬀects are neglected in the material model. The second reason is the very small thickness of the specimen which, combined with its anisotropy, lead to a high sensitivity to non-uniformity in the thickness of the specimens. These eﬀects result in global deformation modes 36 that cannot be captured by the periodicity assumed in our model. In the second case, Vf = 30%, the initial stiﬀness observed in the test lies within the region predicted by the simulations but, once microbuckling takes place, high strains in the matrix would result in localized damage which is, again, not captured by the present model. Overall, the prediction is stiﬀer than the experimental results although much closer than for Vf = 55%. Moment per unit width (N) 0.1 Linear Hexagonal pattern Random pattern Experiments 0.08 0.06 0.04 0.02 0 0 0.05 0.1 0.15 0.2 0.25 0.3 Curvature (mm−1) Figure 25: Comparison of moment vs. curvature in simulations and experiments for Vf = 55%. The plot shows the results from the simulation with hexagonal ﬁber arrangement, the range spanned by the simulations with random RVE, and ﬁve experiments; a linear analysis has been added as a reference. 7. Discussion and Conclusions A composite material consisting of unidirectional carbon ﬁbers embedded in a silicone matrix was fabricated and its bending properties were studied experimentally. It was found that this material can be folded to very high curvatures without any ﬁber damage and its moment vs. curvature relationship is highly non-linear. This behavior is due to the capability of the ﬁbers to micro-buckle within the soft matrix, which provides a stress relief mechanism. Signiﬁcant strain softening was observed when cyclic loading was applied, which 37 Moment per unit width (N) 0.1 0.08 0.06 0.04 Linear Hexagonal pattern Random pattern Experiments 0.02 0 0 0.05 0.1 0.15 0.2 0.25 0.3 Curvature (mm−1) Figure 26: Comparison of moment vs. curvature in simulations and experiments for Vf = 30%. The plot shows the results from the simulation with hexagonal ﬁber arrangement, the range spanned by the simulations with random RVE, and four experiments; a linear analysis has been added as a reference. indicates that, although the ﬁbers appear undamaged, actually some damage is introduced. A ﬁnite element model was created in order to study the micromechanical behavior of thin sheets of this material when it is folded. The model is based on two main simplifying assumptions. The ﬁrst one is the use of a small representative volume element to model a much larger piece of material, using periodic boundary conditions. The ﬁber distribution has been modeled using either a regular hexagonal lattice or a random arrangement based on distributions observed in actual micrographs of the material. The second assumption concerns the behavior of the constituent materials and their interfaces. The ﬁbers were modeled as linear elastic and the matrix as purely hyperelastic; no source of damage or failure was considered and perfect bonding between ﬁbers and matrix was assumed. The model captures the main features that are observed in the folding experiment, including ﬁber microbuckling and the overall nonlinear behavior. When 38 comparing the wavelengths and the moment-curvature relationships between simulations and experiments, the cases with Vf = 30% show good agreement, while in the case of Vf = 55% the ﬁnite element model predicts a shorter wavelength than that observed in experiments. The model also provides a better prediction of the moment vs. curvature relationship for the material with lower volume fraction, although in both cases it is not able to capture the softening observed in the experiments once microbuckling takes place. This disagreement appears to be linked to a key assumption adopted in the material model, namely the lack of any damage or dissipation anywhere. The geometry of the ﬁber composite, coupled with the much higher compliance of the matrix with respect to the ﬁbers, leads to high strain concentrations in the matrix between close ﬁbers. The strains predicted by the present model are much greater than the failure strains measured in uniaxial tests of the matrix, so it is reasonable to assume that the matrix would become damaged before reaching such large strains. This explanation also agrees with the strain softening observed in cyclic tests, which indicates the presence of permanent damage in the material. Observations of the surface of specimens that had been folded to very high curvatures did not show any broken ﬁbers, which suggests that the damage takes place in the matrix or at the interface with the ﬁbers. In conclusion, the present work has shown that very good results can be achieved with a hyperelastic matrix model for the case of low ﬁber volume fraction, although the results are less accurate for composites with a high ﬁber volume fraction. In order to produce a more accurate model for the latter case, it would be necessary to incorporate a damage mechanism able to reduce the strain in the matrix to more realistic values. These issues are beyond the scope of the present study of folding mechanics but a forthcoming paper Lopez Jimenez and Pellegrino (2011) proposes a diﬀerent test that focuses speciﬁcally on the study of nonlinearities due to material damage. 39 Acknowledgements Two anonymous reviewers are thanked for comments on the presentation of this paper. This study was supported with funding from the Keck Institute of Space Studies (KISS) at Caltech and an Earl K. Seals fellowship. The Itochu Corporation of Japan has kindly provided materials for this research. References Abaqus/Standard, 2007. Software, Ver. 6.7, Simulia, Providence, R.I. Adobe Photoshop CS4, 2008. Software, Adobe, San Jose, CA, 2008. Agoras, M., Lopez-Pamies, O., Ponte Castañeda, P., 2009. A general hyperelastic model for incompressible ﬁber-reinforced elastomers. Journal of the Mechanics and Physics of Solids , 268286. Auternaud, J., Bartevian, J., Bertheux, P., Blanc, E., de Mollerat du Jeu, T., Foucras, J., Louis, M., Marello, G., Poveda, P., Roux, C. 1993. SelfMotorized Antifriction Joint and an Articulated Assembly, such as a Satellite Solar Panel, Equipped with such Joints. U.S. Patent 5,086,541.. Barrett, R., Francis, W., Abrahamson, E., Lake, M.S., Scherbarth, M., 2006. Qualiﬁcation of Elastic Memory Composite Hinges for Spaceﬂight Applications, in: 47th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics, and Materials Conference, Newport, Rhode Island, AIAA 2006-2039. Campbell, D., Lake, M., Mallick, K., 2004. A study of the bending mechanics of elastic memory composites, in: 45th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics, and Materials Conference, Palm Springs, CA. Campbell, D., Lake, M., Scherbarth, M., Nelson, E., Six, R.W., 2005. Elastic memory composite material: An enabling technology for future furlable space structures, in: 46th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics, and Materials Conference, Austin, TX. 40 Datashvili, L., Nathrath, N., Lang, M., Baier, H., Fasold, D., Pellegrino, S., Soykasap, O., Kueh, A., Tan, L.T., Mangenot, C., Santiago-Prowald, S., 2005. New concepts and reﬂecting materials for space borne large deployable reﬂector antennas, in: 28th ESA Antenna Workshop on Space Antenna Systems and Technologies, 31 May-3 June 2005, ESTEC, Noordwijk, The Netherlands. Datashvili, L., Baier, H., Wehrle, E., Kuhn, T., Hoﬀmann, J., 2010. Large shellmembrane space reﬂectors, in: 51st AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics, and Materials Conference, Orlando, Florida. Dorfmann, A., Ogden, R.W., 2004. A constitutive model for the Mullins eﬀect with permanent set in particle-reinforced rubber. International Journal of Solids and Structures , 1855–1878. Drapier, S., Garding, C., Grandidier, J.C., Potier-Ferry, M., 1996. Structure eﬀect and microbuckling. Composites Science and Technology 56, 861–867. Drapier, S., Grandidier, J.C., Potier-Ferry, M., 1999. Towards a numerical model of the compressive strength for long ﬁbre composites. European Journal of Mechanics A/Solids 18, 69–92. Drapier, S., Grandidier, J.C., Potier-Ferry, M., 2001. A structural approach of plastic microbuckling in long ﬁbre composites: comparison with theoretical and experimental results. International Journal of Solids and Structures 38, 3877–3904. Fleck, N.A., 1997. Compressive failure of ﬁber composites. Advances in Applied Mechanics 33, 43–117. Francis, W.H., 2008. Mechanics of Post-Microbuckled Compliant-Matrix Composites. Master’s thesis. Colorado State University. Francis, W.H., Lake, M., Steven Mayes, J., 2006. A review of classical ﬁber microbuckling analytical solutions for use with elastic memory composites, 41 in: 47th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics, and Materials Conference, Newport, RI. Fung, Y., 1972. Biomechanics. Mechanical Properties of Living Tissues. Springer, New York. second edition. Gent, A.N., 2005. Elastic instabilities in rubber. International Journal of NonLinear Mechanics 40, 165 – 175. Gent, A.N., Lindley, P.B., 1959. Internal rupture of bonded rubber cylinders in tension. Proceedings of the Royal Society of London—A 249, 195–205. Geymonat, G., Mller, S., Triantafyllidis, N., 1993. Homogenization of nonlinearly elastic materials, microscopic bifurcation and macroscopic loss of rankone convexity. Arch. Rational Mech. Anal. 122, 231–290. Govindjee, S., Simo, J., 1991. A micro-mechanically based continuum damage model for carbon black-ﬁlled rubbers incorporating Mullins’ eﬀect. Journal of the Mechanics and Physics of Solids 39, 87–112. Holzapfel, G.A., Gasser, T.C., Ogden, R.W., 2000. A new constitutive framework for arterial wall mechanics and a comparative study of material models. Journal of Elasticity 61, 1–48. López Jiménez, F., Pellegrino, S., 2009. Folding of thin-walled composite structures with a soft matrix, in: 50th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics, and Materials Conference, Palm Springs, California. López Jiménez, F., Pellegrino, S., 2011. Constitutive modeling of ﬁber composites with a soft hyperelastic matrix. Submitted for publication. Lopez-Pamies, O., Idiart, M.I., 2010. Fiber-reinforced hyperelastic solids: a realizable homogenization constitutive theory. Journal of Engineering Mathematics. 42 Lopez-Pamies, O., Ponte Castañeda, P., 2006. On the overall behavior, microstructure evolution, and macroscopic stability in reinforced rubbers at large deformations: I - application to cylindrical ﬁbers. Journal of the Mechanics and Physics of Solids 54, 831863. Machado, G., Chagnon, G., Favier, D., 2010. Analysis of the isotropic models of the mullins eﬀect based on ﬁlled silicone rubber experimental results. Mechanics of Materials 42, 841–851. Marissen, R., Brouwer, H.R., 1999. The signiﬁcance of ﬁbre microbuckling for the ﬂexural strength of a composite. Composites Science and Technology , 327–330. Mejia-Ariza, J.M., Guidanean, K., Murphey, T.M., Biskner, A., 2010. Mechanical characterization of lgarde elastomeric resin composite materials, in: 51st AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics, and Materials Conference. Mejia-Ariza, J.M., Pollard, E.L., Murphey, T.W., 2006. Manufacture and experimental analysis of a concentrated strain based deployable truss structure, in: 47th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics, and Materials Conference, Newport, Rhode Island. Merodio, J., Ogden, R.W., 2002. Material instabilities in ﬁber-reinforced nonlinearly elastic solids under plane deformation. Archies of Mechanics 54, 525–552. Merodio, J., Ogden, R.W., 2003. Instabilities and loss of ellipticity in ﬁberreinforced compressible non-linearly elastic solids under plane deformation. International Journal of Solids and Structures 40, 4707–4727. Meunier, L., Chagnon, G., Favier, D., Orgéas, L., Vacher, P., 2008. Mechanical experimental characterization and numerical modelling of an unﬁlled silicone rubber. Polymer Testing 27, 765–777. 43 Moraleda, J., Segurado, J., Llorca, J., 2009a. Eﬀect of interface fracture on the tensile deformation of ﬁber-reinforced elastomers. International Journal of Solids and Structures 46, 4287–4297. Moraleda, J., Segurado, J., Llorca, J., 2009b. Finite deformation of incompressible ﬁber-reinforced elastomers: A computational micromechanics approach. Journal of the Mechanics and Physics of Solids 57, 1596–1613. Müller, S., 1987. Homogenization of nonconvex integral functionais and cellular elastic materials. Arch. Rational Mech. Anal. 99, 189–212. Murphey, T.W., Meink, T., Mikulas, M.M., 2001. Some micromechanics considerations of the folding of rigidizable composite materials, in: 42nd AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics, and Materials Conference. NuSil Silicone Technology, March 2007. http://www.nusil.com/library/products/CF19-2615P.pdf. Ogden, R.W., 1972. Large deformation isotropic elasticity - on the correlation of theory and experiment for incompressible rubberlike solids. Proceedings of the Royal Society of London 326, 565–584. Pandolﬁ, A., Holzapfel, G.A., 2008. Three-dimensional modeling and computational analysis of the human cornea considering distributed collagen ﬁbril orientations. Journal of Biomechanical Engineering 130. Pandolﬁ, A., Manganiello, F., 2006. A model for the human cornea: constitutive formulation and numerical analysis. Biomechanics and Modeling in Mechanobiology 5, 237–246. Parnes, R., Chiskis, A., 2002. Buckling of nano-ﬁbre reinforced composites: a re-examination of elastic buckling. Journal of the Mechanics and Physics of Solids 50, 855–879. Ponte Castañeda, P., 2002. Second-order homogenization estimates for nonlinear composites incorporating ﬁeld ﬂuctuations: I - theory. Journal of the Mechanics and Physics of Solids , 737757. 44 Pyrz, R., 1994a. Correlation of microstructure variability and local stress ﬁeld in two-phase materials. Materials Science and Engineering 177, 253–259. Pyrz, R., 1994b. Quantitative description of the microstructure of composites. Part I: Morphology of unidirectional composite systems. Composites Science and Technology 50, 197–208. Rehnmark, F., Pryor, M., Holmes, B., Schaechter, D., Pedreiro, N., Carrington, C., 2007. Development of a deployable nonmetallic boom for reconﬁgurable systems of small spacecraft, in: 48th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics, and Materials Conference, Honolulu, Hawaii. Rimrott, F.P.J., 1966. Storable tubular extendible members. Engineering Digest September, . Rintoul, M., Torquato, S., 1997. Reconstruction of the structure of dispersions. Journal of Colloid and Interface Science 186, 467–476. Rosen, B., 1965. Fiber Composite Materials. Metals Park, Ohio. Schultz, M.R., Francis, W.H., Campbell, D., Lake, M.S., 2007. ysis techniques for shape-memory composite structures, in: Anal48th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics, and Materials Conference, Honolulu, HI. Soykasap, O., 2006. Micromechanical models for bending behaviour of woven composites. Journal of Spacecraft and Rockets 43, (September-October) 10931100. Spencer, A.J.M., 1972. Constitutive theory of strongly anisotropic solids, in: for Mechanical Sciences, I.C. (Ed.), Continuum theory of the mechanics of ﬁbre-reinforced composites. Toho Tenax, retrieved August 2010. http://www.tohotenax.com/tenax/en/products/st_property.php. Watt, A.M., Pellegrino, S., 2002. Tape-spring rolling hinges, in: 36th Aerospace Mechanisms Symposium, NASA Glenn Research Center, May 15-17, 2002. 45 Warren, P. A., 2002. Foldable member. U.S. Patent 6,374,565 B1, April 23 2002. Yee, J.C.H., Soykasap, O., Pellegrino, S., 2002. Carbon ﬁbre reinforced plastic tape springs, in: 45th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics and Materials Conference, Palm Springs, CA, 19-22 April 2004, bibinfolabelAIAA 2004-1819. Yee, J.C.H., Pellegrino, S., 2005. Composite tube hinges. Journal of Aerospace Engineering 18, (October) 224–231. Yee, J.C.H., Pellegrino, S., 2005. Biaxial bending failure locus for woven-thin-ply carbon ﬁbre reinforced plastic structures, in: 46th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics, and Materials Conference, Austin, TX. 46